Research Article High Pressure Elastic Behavior of ... · PDF file on the elastic behavior of...
Embed Size (px)
Transcript of Research Article High Pressure Elastic Behavior of ... · PDF file on the elastic behavior of...
Hindawi Publishing Corporation Advances in Materials Science and Engineering Volume 2013, Article ID 502702, 6 pages http://dx.doi.org/10.1155/2013/502702
Research Article High Pressure Elastic Behavior of Synthetic Mg3Y2(SiO4)3 Garnet up to 9 GPa
Dawei Fan,1 Maining Ma,2 Shuyi Wei,1,3 Zhiqiang Chen,4 and Hongsen Xie1
1 Laboratory for High Temperature and High Pressure Study of the Earth’s Interior of Institute of Geochemistry, Chinese Academy of Sciences, Guiyang 550002, China
2 Key Laboratory of Computational Geodynamics of Chinese Academy of Sciences, University of Chinese Academy of Sciences, Beijing 100049, China
3University of Chinese Academy of Sciences, Beijing 100049, China 4Department of Geosciences, Stony Brook University, Stony Brook, NY 11794, USA
Correspondence should be addressed to Dawei Fan; [email protected]
Received 5 July 2013; Accepted 14 August 2013
Academic Editor: Pavel Strunz
Copyright © 2013 Dawei Fan et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
The compression behavior of synthetic magnesium- (Mg-) yttrium (Y) garnet Mg 3 Y 2 (SiO 4 ) 3 has been investigated upto about
8.79GPa at 300K using in situ angle-dispersive X-ray diffraction and a diamond anvil cell at the beamline X17C, National Synchrotron Light Source, Brookhaven National Laboratory. No phase transition has been observed within the pressure range investigated.The unit-cell parameters and volume decreased systematically with increasing pressure, and a reliable isothermal bulk modulus (𝐾
𝑇0 ) and its pressure derivative (𝐾
𝑇0 ) were obtained in this study. The values of zero-pressure volume 𝑉
0 , 𝐾 0 , and 𝐾
refined with a third-order Birch-Murnaghan equation of state are𝑉 0 = 1727.9 ± 0.2 Å3,𝐾
𝑇0 = 145 ± 3GPa, and𝐾
0 = 8.5 ± 0.9. If𝐾
is fixed at 4, 𝐾 𝑇0
is obtained as 158 ± 2GPa.
Garnets are an important constituent of the uppermantle and mantle transition zone of the Earth and play a fundamental role in high pressure and high temperature petrogenetic processes [1, 2]. Garnets are also important components of subducted oceanic crust, and it is suggested that garnet-rich subducted crust can be gravitationally trapped in the low- ermost part of the mantle transition zone [3–6]. Therefore, accurate knowledge of the physical properties of garnets is essential to infer appropriate compositional models for the upper mantle and mantle transition zone of the Earth. In addition, garnet is the major host of the rare-earth element (REE) both in metamorphic rocks and mantle rocks, and the latter may undergo partial melting in the mantle . Thus, there is a considerable interest in the study of the thermodynamic behavior of REE in garnet that could help to understand the evolution of REE patterns in magmas and in the residual solids [7–9], especially garnets in igneous and metamorphic rocks.
Garnets have the general formula X 3 Y 2 (SiO 4 ) 3 , cen-
tered cubic lattice (space group Ia–3d), and display 8-fold dodecahedral (X), 6-fold octahedral (Y), and tetrahedral (Si) crystallographic sites.This unique behavior makes the garnet structure flexible in accommodating various chemical sub- stitutions with different ionic radii, suggesting that garnets could be composition diverse where X = Mg2+, Fe2+, Ca2+, Mn2+, Y3+; Y = Al3+, Fe3+, Cr3+, and Y3+. Chemical substi- tutions at octahedral and triangular dodecahedral sites may change the relative bond lengths/interatomic distances and angles, which will result in affecting their elastic properties .
Yttrium is a silvery-metallic transition metal chemically similar to the lanthanides, and it has often been classified as a “rare earth element”. Yttrium is almost always found combined with the lanthanides in rare-earthminerals [10, 11]. It is used in the production of a large variety of synthetic garnets , and yttria is used to make yttrium iron garnets (Y 3 Fe 5 O 12 , YIG), which are very effective microwave filters.
2 Advances in Materials Science and Engineering
YIG is also very efficient as an acoustic energy transmitter and transducer . Yttrium aluminium garnet (Y
3 Al 5 O 12 , YAG)
is used in a number of industrial applications, either in the pure phase form or as a composite .
To date, the elastic properties of pyrope have been studied extensively by multianvil apparatus and diamond anvil cell [6, 15–22]. However, nowadays, there are no studies available on the elastic behavior of rare-earth silicate garnet at high pressure. In addition, yttrium not only can substitute for Mg at the dodecahedral site but also can substitute for Al at the octahedral site in the silicate garnet. In this paper, we report the elastic measurements of magnesium- (Mg-) yttrium (Y) garnet [Mg
3 Y 2 (SiO 4 ) 3 ], a synthetic rare-earth silicate garnet,
up to pressures of 8.79GPa at room temperature. Along with the previous results for pyrope [6, 15–22], the compositional dependence of the bulk modulus is discussed.
2. Sample and Experiment
The Mg 3 Y 2 (SiO 4 ) 3 sample used in our high pressure pow-
der X-ray diffraction experiments was synthesized with a multianvil pressure apparatus (YJ-3000T) installed at the Institute of Geochemistry, Chinese Academy of Sciences. Details about the apparatus have been described by Xie et al. . The pressurization system of this press consists of six WC anvils, with their tips truncated as 23.5 × 23.5mm2, which are simultaneously pushed by six hydraulic rams so that high pressure is generated in the experimental assembly. The experimental assembly, YJ-3000T, used in this study, is schematically illustrated in Figure 1. The experimental temperature was measured and controlled with a Pt
94 Rh 6 -
Pt 70 Rh 30 thermocouple (type B). The starting materials used
in the synthesizing experiments were stoichiometric amounts of high purity MgCO
3 , Y 2 O 3 , and SiO
2 and were placed
one night at 800∘C for removing carbonates. The mixture was then melted at 1400∘C which produced, after quenching, a homogeneous glass. The homogeneous glass was crushed into a fine powder using acetone. The starting mixtures were encapsulated in platinum capsules.The synthesizing pressure and temperature conditions were 4GPa and 1000∘C for 24 h. The crystal structure of sample was confirmed by using pow- derX-ray diffractionmethod (X’Pert ProMPD system).Their compositions were confirmed by using electron microprobe analysis (EPMA-1600).
In this investigation, we conducted in situ high-pressure angle dispersive X-ray diffraction experiments at the beam- line X17C, National Synchrotron Light Source (NSLS), Brookhaven National Laboratory, using a 0.37677 Å X-ray beam and CCD detector, and the beamline 4W2, Beijing Synchrotron Radiation Facility (BSRF), using a 0.6199 Å X- ray beam and Mar345 detector. We generated the high pres- sure by using a symmetrical diamond-anvil cell, equipped with two diamonds anvils (culet face diameter: 500 𝜇m) and tungsten-carbide supports. In these high pressure experi- ments, T301 stainless steel plates with an initial thickness of 200𝜇m were used as gaskets, with their central part preindented to a thickness of about 50 𝜇m and then drilled through into a hole of 200𝜇m diameter. The finely ground
Sample Pyrophyllite Alumina Magnesium
Heater Thermocouple and insulating tube
Figure 1: Experimental assembly used in the high pressure syn- thesizing experiments with a multianvil pressure apparatus (YJ- 3000T) installed at the Institute of Geochemistry, Chinese Academy of Sciences.
Mg 3 Y 2 (SiO 4 ) 3 powder, plus a couple of tiny ruby balls
together with a methanol : ethanol : water mixture (16 : 3 : 1 by volume) which is a hydrostatic pressure-transmitting medium up to about 10GPa , was loaded into the gasket hole. The ruby fluorescence method  was employed to determine the experimental pressure. The X-ray diffraction patterns (collecting time = 10min) were integrated to gener- ate the conventional one-dimensional profiles using the Fit2D program . The sample was equilibrated for about 10min before diffraction data measurement, and subsequently the pressure was raised up to 8.79GPa. Unit-cell parameters were refined by Le Bail fitting using the GSAS package [27, 28] and user interface EXPGUI  up to 8.79GPa (Table 2). Backgroundwas fitted using theChebyschev polynomial, and X-ray peak shapes were fitted using the pseudo-Voigt profile function proposed byThomson et al. .
3. Result and Discussion
The powder X-ray diffraction data of Mg 3 Y 2 (SiO 4 ) 3 at ambi-
ent conditions revealed that this phase has a cubic structure (Ia–3d), with unit-cell dimensions of 𝑎 = 11.9995(4) Å. The observed and calculated X-ray diffraction patterns of Mg 3 Y 2 (SiO 4 ) 3 at ambient conditions are listed in Table 1.The
volume of Mg 3 Y 2 (SiO 4 ) 3 unit cell at ambient conditions is
1727.8(2) Å3. The high pressure X-ray diffraction data were collected
up to 8.79GPa at ambient temperature. Typical X-ray diffrac- tion spectrums at selected pressure is shown in Figure 2. The diffraction patterns at each pressure of the study are
Advances in Materials Science and Engineering 3
Table 1: Observed and calculated X-ray diffraction patterns of Mg3Y2